Jun 22, 2017 - However, their near- and far-field properties in most cases ... line width and spectral position of the far-field and near-field resonances of ST- ...
Jun 22, 2017 - Lithographic and nonlithographic two-dimensional (2D) substrates for surface-enhanced Raman spectroscopy (SERS) have gained enormous popularity as analytical platforms for detection and identification of various analytes. However, thei
Jun 22, 2017 - ... which is jointly supported by the Office of the Provost, the Office for Research, and Northwestern University Information Technology (NUIT).
Department of Physics & Astronomy, The University of Texas at San Antonio, One ... electron microscopy FONs fabricated by either stationary (ST-FONs) or spun ...
Farfield Tracing of a Point Source Discharge Plume in the Coastal Ocean Using Sulfur ... Nova Southeastern University, 8000 North Ocean Drive, Dania Beach, ...
Dec 12, 2016 - Microbial Biotechnology and Protein Research Laboratory, Department of Molecular Biology and Biotechnology, Tezpur University,. Tezpur ...
Oct 15, 2018 - College of Chemistry and Materials Science, Guangxi Teachers Education University, Nanning 530001, Guangxi, P. R. China. â¢S Supporting ...
Dec 12, 2016 - The proteome composition of western India (WI) Russell's viper venom ... For a more comprehensive list of citations to this article, users are ...
Jul 27, 2016 - to 10 mL/h, fraction volume was 2.0 mL, and protein elution was monitored at ..... (Amersham Bioscience, UK) at 20 mA (1.2 mA/cm2) for 2 h. The transfer ... NBT kit (Sigma-Aldrich, USA) and scanned using an EPSON scanner, and ..... pro
Feb 9, 2017 - We report the measurement of the binding constants (Ka) for cucurbit[n]uril (n = 7, 8) toward four series of guests based on 2,6-disubstituted adamantanes, 4,9-disubstituted diamantanes, 1,6-disubstituted diamantanes, and 1-substituted
Subscriber access provided by EAST TENNESSEE STATE UNIV
Unraveling Near- and Far-Field Relationship of 2D SERS Substrates Using Wavelength-Scanned SurfaceEnhanced Raman Excitation Spectroscopy (WS-SERES) Dmitry Kurouski, Nicolas Large, Naihao Chiang, Anne-Isabelle Henry, Tamar Seideman, George C. Schatz, and Richard P. Van Duyne J. Phys. Chem. C, Just Accepted Manuscript • DOI: 10.1021/acs.jpcc.7b04787 • Publication Date (Web): 22 Jun 2017 Downloaded from http://pubs.acs.org on June 24, 2017
Just Accepted “Just Accepted” manuscripts have been peer-reviewed and accepted for publication. They are posted online prior to technical editing, formatting for publication and author proofing. The American Chemical Society provides “Just Accepted” as a free service to the research community to expedite the dissemination of scientific material as soon as possible after acceptance. “Just Accepted” manuscripts appear in full in PDF format accompanied by an HTML abstract. “Just Accepted” manuscripts have been fully peer reviewed, but should not be considered the official version of record. They are accessible to all readers and citable by the Digital Object Identifier (DOI®). “Just Accepted” is an optional service offered to authors. Therefore, the “Just Accepted” Web site may not include all articles that will be published in the journal. After a manuscript is technically edited and formatted, it will be removed from the “Just Accepted” Web site and published as an ASAP article. Note that technical editing may introduce minor changes to the manuscript text and/or graphics which could affect content, and all legal disclaimers and ethical guidelines that apply to the journal pertain. ACS cannot be held responsible for errors or consequences arising from the use of information contained in these “Just Accepted” manuscripts.
Unraveling Near- and Far-Field Relationship of 2D SERS Substrates Using Wavelength-Scanned Surface-Enhanced Raman Excitation Spectroscopy (WS-SERES). Dmitry Kurouski†*, Nicolas Large‡, Naihao Chiang, Anne-Isabelle Henry, Tamar Seideman, George C. Schatz, and Richard P. Van Duyne* Department of Chemistry, Northwestern University, 2145 Sheridan Road, Evanston, Illinois 60208, United States *E-mail: [email protected]; [email protected] Current addresses: † Department of Biochemistry and Biophysics, Texas A&M University, 300 Olsen Blvd, College Station, Texas 77843, United States. ‡ Department of Physics & Astronomy, The University of Texas at San Antonio, One UTSA Circle, San Antonio, Texas 78249, United States. ABSTRACT: Lithographic and non-lithographic two-dimensional (2D) substrates for surface-enhanced Raman spectroscopy (SERS) have gained enormous popularity as analytical platforms for detection and identification of various analytes. However, their near- and far-field properties in most cases remain poorly understood. We have previously developed a metal nanopillar film over nanospheres (FON) platform exhibiting Raman enhancement factors ~107. These substrates have a reproducible and predictable localized surface plasmon resonance (LSPR) throughout the entire visible and much of the near-IR regions of the electromagnetic spectrum. Extending upon these results, we have utilized wavelength-scan surface-enhanced Raman excitation spectroscopy (WS-SERES) to unravel the relationship between near- and far-field properties of FON SERS substrates. We examined by scanning electron microscopy FONs fabricated by either stationary (ST-FONs) or spun (SP-FONs) metal deposition to examine the interrelationships of nanoscale structure, near- and far-fied properties. We demonstrate that the linewidth and spectral position of the far-field and near-field resonances of ST- and SP-FONs directly depends on the nanofeature distribution at the metallic surface. In particular, we show that the actual nanofeature morphology and distribution directly impact the spectral alignment of the farfield and near-field resonances.
INTRODUCTION Surface-enhanced Raman spectroscopy (SERS) is a powerful analytical technique that is capable of detecting molecular analytes down to the single molecule level.1,2 Electromagnetic enhancement is demonstrated to be the dominant mechanism contributing to the SERS enhancement.3 It involves the localization and amplification of the incident optical excitation by surface plasmon resonances (localized and propagating) of noble metal nanoparticles.4-7 Localized surface plasmon resonances (LSPRs) are coherent, incompressible, collective oscillations of the conduction electron gas sustained by noble metal
nanoparticles and nanostructured surfaces. They are responsible for drastic enhancement of the local electric field (E) in the vicinity of the metallic nanofeatures, which can reach 102−103 times of the incident electric field (E0).8 The LSPR strongly depends on plasmonic nanofeature size, shape, material, and local dielectric environment.9-13 Therefore, in principle, the knowledge of the LSPR spectral properties, which can be obtained from the far-field scattering spectrum, should be sufficient to determine the excitation wavelength that would give the highest enhancement factor (EF~|E/E0|4) for a given SERS substrate. Chemically synthesized gold and silver nanoparticles have been routinely used for single-molecule SERS experiments, where their aggregation into nanoparticle clusters provides the sites for electromagnetic field enhancement, also known as hot-spots.14-17 Nanoparticle synthesis is versatile, allowing for tailoring the sizes and geometries of the nanoparticles to fulfill particular experimental needs.18-22 Recently, numerous different kinds of nanoparticles with built-in hot-spots, i.e. eliminating the need for nanoparticle aggregation, have been reported. They include porous nanoparticles, octopods/nanostars, octahedra, concaved-, truncated-, and etched-nanocubes, and nanocuboids.18,22-26 However, nanoparticle synthesis scale-up can be difficult to implement and often results in an increase of the size polydispersity. Furthermore, precursors of their synthesis, such as cetyltrimethylammonium bromide (CTAB) and citric acid, commonly overcomplicate their practical applications in surface-enhanced spectroscopies and sensing.9,27 Removal of these surfactants commonly leads to random aggregation and precipitation of the metallic nanoparticles, which prevents reproducibility of the resulting SERS enhancement. Two-dimensional (2D) SERS substrates are ideally suited platforms for the detection of analytes as they provide adequate nanofeatures without the need for stabilizing adsorbants that could in fine limit the SERS efficiency by blocking the analytes’ access to the metal surface. The bare metallic nanostructured film can then potentially be later functionalized with specific capture ligands.28,29 Over the last decades, several SERS substrates have been proposed, including film over nanospheres (FON),30,31 colloidal crystals films,32 nanoparticle arrays,33-38 particles grafted on silanized glasses,39,40 paper-based 3D SERS substrates,41 and plasmonic nanoholes.18,22,26,42 Based on the fabrication techniques used, there are several types of SERS platforms. The fabrication of non-lithographic substrates is commonly carried out through a thermal evaporation of plasmonic metals on a glass or silicon substrate.43 This results in generation of nanometer-scale plasmonic features.44,45 Although the fabrication of non-lithographic substrates such as metal islands or porous films is relatively facile and provide reasonable SERS enhancement (104–106), the lack of control in the density of hot-spots on the substrate makes it difficult to use as a reliable substrate. Lithographic substrates are characterized by well-defined nanostructures at specific locations on the substrate and hence to achieve high SERS enhancement factors (typically, 106−108).46-48 Electron-beam lithography (EBL) is one of the commonly used methods to fabricate nanoparticle arrays with tunable interparticle distances and shapes.49,50 However, high labor intensity and time consumption of EBL-based substrates and high fabrication costs limit their broad and large scale utilization.48 A welldeveloped type of lithographic substrate is the FON, which is fabricated by metal evaporation on a mask of close-packed silica or polystyrene spheres.30,31,47 It was previously demonstrated that LSPR of FONs could be tuned between 330 and 1840 nm by varying the diameter of the silica or polystyrene spheres. Moreover, FONs exhibit one of the highest reported EF of 108 with only 10% variability over substrates of 10 cm in diameter. It was also noted that as a result of metal deposition over the close-packed silica or polystyrene spheres, two major types of nanofeatures are grown: elongated nanopillars and nanoscale
blobs. Greeneltch et al. showed that substrate spinning during the metal deposition promotes the formation of nanopillars.51 These spun FON substrates (SP-FONs) exhibited EF nearly an order of magnitude higher than FONs prepared under stationary conditions (ST-FONs). However, it remains unclear how different is the distribution of nanofeatures, and how their size, shape, and overall morphology affect the relationship between near- and far-field properties of these FON substrates. The morphological differences in a SERS substrate family can leads to complex near- to far-field relationships.41 Elucidation of such relationships allows for even more precise tuning and tailoring of the LSPR of the FON substrate, thus leading to a better optimization of its SERS performance. Wavelength-scan surface-enhanced Raman excitation spectroscopy (WS-SERES) is capable of unraveling near-field properties of SERS substrates. Using WS-SERES, Doherty et al. previously demonstrated that highly uniform SERS substrates exhibit ~50 nm red-shift of their near-field maximum compared to the maximum of their optical scattering profile.33 McFarland et al. observed that near- and far-field profiles of periodic particle arrays (PPAs) would overlap if the substrate was annealed at 300 °C for one hour.52 Finally, WS-SERES was recently used to investigate near-field properties of paper- and fabric-based 3D SERS substrates, which demonstrated extremely weak optical scattering.41 It was found that nanoparticle dimers, trimers, and higher order nanoparticle clusters primarily determine the near-field properties of these substrates. It should be noted that SERS signals are mainly generated at hotspots at plasmonic substrates; thus, SERS excitation spectral shapes are considerably affected by near-field optical profiles of hotspots that are different from the far-field optical profiles of the overall plasmonic substrates. At the same time, the far-field response of 3D SERS substrates was shown to either primarily originate from the monomers or could not be clearly defined. In the present study we have utilized WS-SERES, scanning electron microscopy (SEM), optical scattering, and finite-difference time-domain (FDTD) calculations to explore near- and far-field properties of FON substrates. Specifically, we unravel the effect of the FON nanofeature distributions on the correlation between the near- and far-field responses of these SERS substrates. We noticed that spun deposition of Ag resulted in the predominant formation of nanopillars on the surface of the FONs. On the other hand, stationary deposition of Au led to near exclusive growth of nanoscale blobs. Here, we used these peculiarities of metal deposition to promote the growth of two different kinds of nanofeatures, i.e., nanopillars (SP-FON) and nanoscale blobs (ST-FON), on the surface of FONs. New structural models of both FON structures have been developed, and electrodynamics calculations are used with these models to provide a quantitative description of the observed optical properties. METHODS: Fabrication of SERS substrates. Both SP- and ST-FON SERS substrates were prepared by packing silicon spheres (600 and 540 nm, respectively) on freshly cleaned silicon wafers, as previously described in Ref. 51. 200 nm of Ag was deposited on the spheres while the substrates were spun at ~550 rpm (home-made thermal evaporator) for the SP-FONs. ST-FONs were prepared by evaporation of 150 nm of Au on stationary hold substrates (PVD 75, Kurt J. Lesker, Efferson Hills, PA, USA). Benzenethiol (Sigma-Aldrich, St. Louis, MO, USA) was vapor-deposited onto the ST- and SP-FON SERS substrates by placing 3−4 drops of concentrated (100%) benzenethiol solution in a Petri dish around the substrate. Substrates were left overnight in the atmosphere of benzenethiol vapors and measured using WS-SERES immediately after.
Cyclohexane (Sigma-Aldrich, St. Louis, MO, USA) was used as an intensity standard (1028.3 cm-1 normal Raman scattering band) for a correction of the inherent ν4 behavior of Raman scattering. Specifically, the intensity of the 1075 cm-1 band of benzenethiol, which was used as a reported of SERS signal for all substrates, was divided by the intensity of the 1028.3 cm-1 band of cyclohexane to obtain the SERS efficiency at each excitation wavelength. Such normalization also allows us to eliminate variations in the SERS intensity that are not due to enhancement by the substrate, as well as the spectral dependence of the detection system.52 Raman Spectroscopy. SERS and normal Raman spectra were collected on an inverted microscope (Nikon TE-300) equipped with a 20X dry Nikon objective (NA=0.45) from the same area of the SERS substrate as the reflection spectra were captured from. A diode pumped solid-state laser Spectra-Physics (Mountain View, CA, USA) Millenia Xs was used for 532 nm excitation. It was also used to drive the tunable Ti:Sapphire oscillator to generate wavelengths from 725 to 825 nm. Spectra-Physics He-Ne diode-based laser was used to generate a 633 nm laser excitation. The laser spot size was approximately 2.7 µm x 1.8 µm. The signal was collected in a backscattering configuration and directed to a confocal Raman spectrometer (Princeton Instruments, SP2500i) equipped with a 1200 groove/mm grating blazed at 500 nm (532 nm excitation) or 600 groove/mm grating blazed at 750 nm (633, 725−825 nm excitations) and a slit entrance set to 100 µm. Prior to entering the spectrograph Rayleigh scattering was filtered with a long-pass filter (Semrock, LP03−532RS-25 (532 nm excitation) or LP03−633RS-25 (633 nm excitation)). To filter the Rayleigh scattering at 725−825 nm excitations, a 900/11 nm VersaChrome tunable band-pass filter was used. The dispersed light was then sent to a liquid nitrogen-cooled CCD (Action300i, Spec-10 400B). A motorized stage (Physik Instrumente, 710 Digital PZT) was used to move the sample relative to the incident laser beam. All data was processed using GRAMS/AI 7.0 (Thermo Galactic, Salem, NH, USA). UV-Vis Spectroscopy. Scattering spectra (400−900 nm) were recorded by illuminating the sample with the microscope lamp and analyzing the transmitted light by a fiber-optically coupled Ocean Optics spectrometer (SD200, Ocean Optics, Dundein, FL, USA).5147The size of the light spot was approximately 1 mm in diameter. The spot to spot variations in the reflectance were negligible (Figure 1S). Taqu=10 ms and 103 averages. Silver and gold films with the same metal thickness as was deposited on the investigated substrates were used as a reference to reach 100% transmission. Scanning Electron Microscopy. Scanning electron microscopy (SEM) images were acquired with a LEO Gemini 1525 microscope using an InLens detector, operating at an acceleration voltage of 5.00 kV. The working distance was varied between 3 and 7 mm. Electrodynamic Calculations. Finite-difference time-domain (FDTD) simulations were performed using the commercial package Lumerical FDTD Solutions53 to calculate the plasmonic properties (reflectance and near-field) of the FON substrates. The FONs were modeled based on the SEM data. The silica spheres are modeled with diameters of 600 and 540 nm for the ST-FON and SP-FON, respectively, and are arranged in a hexagonal lattice on a semi-infinite silica substrate. The ST-FON is modeled with a 200 ±10 nm metallic layer constituted of approximately 3,000 elongated spheroids of sizes ranging from 5 to 20 nm randomly distributed on top of each microsphere. Similarly, the SP-FON is modeled with a 150 ±10 nm metallic layer constituted of ~3,000 randomly distributed 15−20 nm spherical grains. The two FDTD-modeled geometries are shown in Figure 3. Periodic boundary conditions and symmetries
were used in the in-plane directions to mimic infinite arrays and perfectly-matched layers (PMLs) were assumed along the out-of-plane direction. Dielectric permittivities tabulated by Palik and by Johnson and Christy were used for Ag and Au, respectively.54,55 The optical excitation was taken as a broad-band plane-wave source (total-field scattered-field, TFSF source). A non-uniform conformal mesh with a minimum mesh size of 0.25 nm was used to describe the overall nanostructures. An auto-shutoff parameter of 10-6 was chosen as convergence parameter, allowing a propagation time τ~10 ns of the electromagnetic fields. The reflectance spectra are averaged over 15 different morphologies (i.e., nanofeature distributions) to account for experimental heterogeneities. RESULTS AND DISCUSSION Electron microscopy examination provides a mean to evaluate the structural uniformity of a substrate, as well as providing information about the size and shape of the observed nanofeatures. This information is commonly used as an input for theoretical and numerical calculations of the substrate near- and far-field properties. We used scanning electron microscopy (SEM) to examine the morphology of the nanostructured metal film and characterize the shape and sizes of the nanofeatures present at the surface of both ST- and SP-FONs (Figure 1). The morphological analysis reveals that SP-FONs had average feature sizes of 24 ± 5 and 22 ± 5 nm with full-width half-maximum (FWHM) of 10 nm in top and side view, respectively. As for the other substrates, namely ST-FONs, average nanofeature sizes of 28 ± 11 and 47 ± 16 nm with FWHM of 20 and 70 nm were observed in top and side view, respectively. From these data on the side and top views, nanofeatures on ST-FONs appear very asymmetric (28 and 47 nm, respectively), in contrast to their counter-parts on the SP-FONs (24 and 22 nm, respectively).
Figure 1. SEM images of SP-FONs (A, B) and ST-FONs (C, D). Scale bars correspond to 200 nm (A, B) and 300 nm (C, D). (E) Size distributions of nanofeatures on the top (upper panels) and side (lower panels) surface of SP- and ST-FONs. We further characterized the SP-FONs and ST-FONs by measuring their both near- and far-field responses. The near-field SERS response was measured using WS-SERES from nine different, nonoverlapping spots on three SP-FON and two ST-FON substrates. The excitation wavelength employed in all the measurements was tuned from 725 to 825 nm, in increments of 10 nm (Figure 2). Benzenethiol (BZT, inset Figure 2A) was used as the probed analyte because it forms a monolayer on the metal surface and is not resonant in 600-900 nm spectra window. Overnight exposition of ST- and SP-FON substrates in the atmosphere of BZT results in the formation of a BZT monolayer on the metal surface. A typical SERS spectrum obtained from such metallic surface is shown in Figure 2A (black line). It should be noted that the SERS spectra of BZT acquired from ST-FONs and SP-FONs are very similar to each other. A normal Raman spectrum of BZT is also shown for comparison (Figure 2A, red line). Finally, the
Both ST- and SP-FONs exhibit Gaussian near-field profiles with the maxima around 755-775 nm. STFONs (Figure 2B) showed nearly similar enhancement in the 750−790 nm range (EF≈8.3×106). We also found that the EF of ST-FONs decreased by nearly a factor of two at 725 and 825 nm relative to the maximum, giving rise to a FWHM of ~75 nm, slightly broader than their SP-FON counter-parts (FWHM of ~65 nm, Figure 2C). The highest enhancement is found at 755−775 nm, which corresponds to EF≈1×107. The second largest enhancements were measured at 745, 785, and 795 nm (EF≈8.3×106). Finally, the lowest EF for SP-FONs was observed at 725 nm (EF≈2×106). The far-field properties exhibit opposite behaviors as shown by the reflectance spectra (Figure 2B,C, dotted lines). The spectrum of the SP-FON substrates appears to be broader than the scattering profile of ST-FONs (FWHM of 160 vs. 110 nm). Interestingly, we can also notice that the maxima for the far-field scattering and for the near-field response are spectrally aligned in the case of the SP-FONs (Figure 2C). On the other hand, the maximum of the near-field response of the ST-FON is red-shifted by about 45 nm with respect to the reflectance (far-field) maximum (Figure 2B). In order to gain further insight into the structure-properties relationships of the FON substrates and further understand the relationship between the near- and far-field properties, we have used the finite-difference time-domain (FDTD) method to calculate the near- and far-field properties of both ST- and SP-FONs (Figure 3A and B, respectively). Due to the structural complexity of these substrates, FDTD calculations were performed for 15 different morphologies (i.e., different surface roughness distributions) and averaged out. The far-field optical properties are also polarization averaged. The simulation details are provided in the method section. As the SERS signal is experimentally dominated by strong plasmonic hot-spots present at the surface of the metallic nanostructured film, we calculate the near-field response in the gap regions, i.e., where the local electric field intensity is the highest (white mark in Figure 3E and F). Similarly to the experimental results, we have found that the maximum of the near-field response (i.e., max(|E/E0|4)) of the ST-FON is red-shifted by ~60 nm with respect to the reflectance minimum, as shown in Figure 3C. However, the SP-FON does not exhibit such noticeable spectral shift as it can be seen from Figure 3D. Instead, near- and far-field profiles of SP-FON appeared to be spectrally aligned as observed experimentally. Additionally, and very similarly to the experimental observations, the reflectance profile of Ag SP-FONs appears much broader than that of Au ST-FONs. These results are in excellent quantitative agreement with the WS-SERES results presented in Figure 2. Note also that the maximum experimental and calculated enhancements for both ST-FON and SP-FON are similar, and are on the order of 106-7. It is important to notice that although the morphology is modeled with random surface roughness, small discrepancies in the spectral line-shape can be attributed to high surface heterogeneity of the actual FONs, thus leading to large inhomogeneous spectral broadening. Figure 3E and F shows the near-field spatial distribution (|E/E0|4) at the LSPR resonance (i.e., when the local electric field is the most intense). It can be seen that most of the near-field is located in the gaps between the microspheres. However, due to the surface roughness, some localized hot-spots can be found on top of the FON, in particular for the Ag SP-FON (Figure 3F). This is in agreement with previous published work on the distance dependence of SERS.56 As it can be seen from Figure 3C-F, the calculated EF reaches values of the order of 3×106, very good quantitative agreement with the experimental estimations.
Figure 3. FDTD calculations for the ST- and SP-FONs. (A, B) Modeled geometries used in the FDTD simulations for the Au ST-FON and Ag SP-FON, respectively. (C, D) Reflectance spectra (dotted lines) and fourth power of the near-field (|E/E0|4, solid line) calculated within the gap (white mark in panels E and F) for the Au ST-FON and Ag SP-FON, respectively. (E, F) Spatial distribution of |E/E0|4 around the Au ST-FON (λ=810 nm) and Ag SP-FON (λ=800 nm), respectively. In order to demonstrate that the observed relationship between near- and far-field responses is not due to a
nature of the plasmonic metal used in each of the investigated FON we have performed the same theoretical analysis with the complementary configurations. Specifically, we calculated the near- and farfield properties of Au SP-FONs and Ag ST-FONs (Figure 4A and B). As it can be clearly noticed from Figure 4D, the maximum of the near-field response (max(|E/E0|4)) of Ag ST-FON, similarly to the Au ST-FON in Figure 3, is red-shifted by about 50 nm with respect to the reflectance minimum. At the same time, both Au SP-FONs do not exhibit such a spectral shift (Figure 4C).
Figure 4. FDTD calculations for the SP- and ST-FONs. (A, B) Modeled geometries used in the FDTD simulations for the Au SP-FON and Ag ST-FON, respectively. (C, D) Reflectance spectra (dotted lines) and fourth power of the near-field (|E/E0|4, solid line) calculated within the gap (white mark in panels E and F) for the Au SP-FON and Ag ST-FON, respectively. (E, F) Spatial distribution of |E/E0|4 around the Au SP-FON (λ=700 nm) and Ag ST-FON (λ=725 nm), respectively.
Unraveling the relationship between the far- and near-field optical responses of plasmonic materials is important to further understand the role and control the fabrication of nanoscale features underlying the SERS effect, as well as for the rational fabrication of SERS substrate and ultimately the optimization of their performance. However, to date, the interrelationship between nanoscale morphology of 2D substrates such the ones found in the metal film of FONs and their properties was not clearly understood. Due to the intrinsic structural heterogeneity of these substrates at the nanoscale, the prediction of their optical far- and near-field properties using theoretical models is challenging. In the current study we demonstrated that SEM allows for the visualization of morphological heterogeneity of nanostructures on the surfaces of both ST- and SP-FONs. However, these results alone cannot be used for prediction of farand near-field properties of FONs. For instance, according to the SEM images, nanopillars on the surface of SP-FON are 25−30 nm in diameter. However, such nanofeatures would exhibit LSPR at ~500 nm, which was not experimentally observed.57,58 Similarly, the size of the ST-FONs nanofeatures (28-47 nm) should give rise to a much broader far-field optical response than the optical response of SP-FONs (nanofeatures of 25−30 nm in diameter). However, direct measurements of the optical scattering from STand SP-FONs showed the opposite (Figure 2), which is also supported by the FDTD calculations (Figures 3 and 4). From the two set of FDTD calculations it clearly appears that the spectral shift observed experimentally with the ST-FONs (Figure 2B), or the spectral alignment observed with ST-FONs (Figure 2C), is directly connected to the actual morphology of the FON rather than to the material. Spectral red-shift between near-field and far-field resonances is commonly observed in plasmonic nanostructures. Using coupled
harmonic oscillator models, Zuloaga and Nordlander showed that the amount of red-shift varies based on the total damping in the system.59 Besides the intrinsic damping of the plasmonic materials, the total damping is directly governed by the type of morphological features forming the nanostructure (radiative damping). Small particles, or in the case of the ST-FONs small nanofeatures (i.e., nanopillars), have minimal radiative damping and very little intrinsic damping, resulting in a negligible (or absence of) redshift of the near-field spectrum. As for SP-FONs, the small blobs tend to merge more easily than the nanopillars and form smoother and more continuous metallic films, thus resulting in overall larger features as it can be seen in the FDTD models (Figures 3A and 4B). This effect further results in a significant increase of the radiative damping due to prominent retardation effects, leading to important spectral shifts. Furthermore, the actual size distribution of these nanofeatures also directly impacts the inhomogeneous damping of the system. CONCLUSIONS: In conclusion, we unraveled the interrelationships between the structure, near- and far-field properties of SERS substrates made of nanostructured metal film over nanospheres, known as FONs. Depending on the fabrication method (stationary vs spinning metal deposition, designated as ST-FONs and SP-FONs, respectively), we clearly confirmed by SEM analysis that it is possible to control the fine morphology of the metal film in the 10-90 nm range, with the resulting nanofeatures differ in their shape and size dispersity. Using WS-SERES, we directly measured the near-field SERS enhancement profile of both STFONs and SP-FONs and clearly showed that the near- and far-field profiles of SP-FONs were spectrally aligned, whereas a ~45 nm spectral shift was observed in the case of ST-FONs. The extensive numerical analysis revealed that the presence of nanofeatures presenting a small size polydispersity results in the spectral alignment of optical far-field and near-field profiles. The absence of, commonly observed, nearto far-field spectral shift is attributed to a significant increase in the radiative damping originating from the surface morphology of the FONs.
AUTHOR INFORMATION Corresponding Author *Richard P. Van Duyne, [email protected]; Dmitry Kurouski, [email protected] Author Contributions D.K and N.C. conceived and designed the experimental measurements. A.-I.H. performed the SEM structural analysis. N.L. performed the electrodynamic calculations and theoretical analysis. The manuscript was written through contributions of all authors. All authors have given approval to the final version of the manuscript. ACKNOWLEDGEMENTS This work made use of the EPIC facility of Northwestern University’s NUANCE Center, which has received support from the Soft and Hybrid Nanotechnology Experimental (SHyNE) Resource (NSF ECCS-1542205); the MRSEC program (NSF DMR-1121262) at the Materials Research Center; the
International Institute for Nanotechnology (IIN); the Keck Foundation; and the State of Illinois, through the IIN. This work was also supported by the NSF CaSTL Center (NSF grant CHE-1414466) and by AFOSR MURI grant FA9550-14-1-0003. N.L. acknowledges financial support from the Department of Physics and Astronomy and from the College of Science of the University of Texas at San Antonio. Computing resources were provided by the Quest high performance computing facility at Northwestern University which is jointly supported by the Office of the Provost, the Office for Research, and Northwestern University Information Technology (NUIT). This material is also based on research sponsored by the Air Force Research Laboratory under agreement FA8650-15-2-5518. The U.S. Government is authorized to reproduce and distribute reprints for Governmental purposes notwithstanding any copyright notation thereon. The views and conclusions contained herein are those of the authors and should not be interpreted as necessarily representing the official policies or endorsements, either expressed or implied, of Air Force Research Laboratory or the U.S. Government. Finally, this work was supported by the Assistant Secretary of Defense for Health Affairs, through the Peer Reviewed Medical Research Program under Award No. W81XWH-16-1-0375. Opinions, interpretations, conclusions and recommendations are those of the author and are not necessarily endorsed by the Department of Defense. Supporting Information Available: the spot to spot variations in the reflectance spectra of SP-FON are shown in Figure S1. This information is available free of charge via the Internet at http://pubs.acs.org
REFERENCES (1) Kneipp, K.; Wang, Y.; Kneipp, H.; Perelman, L. T.; Itzkan, I.; Dasari, R. R.; Feld, M. Single Molecule Detection Using Surface-Enhanced Raman Scattering (SERS). Phys. Rev. Lett. 1997, 78, 1667-1670. (2) Nie S; Emory, S. R. Probing Single Molecules and Single Nanoparticles by SurfaceEnhanced Raman Scattering. Science 1997, 275, 1102-1106. (3) Schatz, G. C.; Yong, M. A.; Van Duyne, R. P.: Electromagnetic Mechanism of SERS. In Surface-Enhanced Raman Scattering: Physics and Applicaitons; Kneipp, K., Moskovits, M., Kneipp, H., Eds.; Springer, Berlin, 2006; Vol. 103; pp pp. 19-46. (4) Moskovits, M. Surface Roughness and the Enhanced Intensity of Raman Scattering by Molecules Adsorbed on Metals J. Chem. Phys. 1978, 69, 4159-4161. (5) Gersten, J.; Nitzan, A. Electromagnetic Theory of Enhanced Raman-Scattering by Molecules Adsorbed on Rough Surfaces. J. Chem. Phys. 1980, 73, 3023-3037. (6) Kerker, M.; Wang, D. S.; Chew, H. Surface Enhanced Raman Scattering (SERS) by Molecules Adsorbed at Spherical Particles. Appl. Opt. 1980, 19, 3373-3388. (7) King, F. W.; Van Duyne, R. P.; Schatz, G. C. Theory of Raman Scattering by Molecules Adsorbed on Electrode Surfaces. J. Chem. Phys. 1978, 69, 4472-4481. (8) Hao, E.; Schatz, G. C. Electromagnetic Fields Around Silver Nanoparticles and Dimers. J. Chem. Phys. 2004, 120, 357-366. (9) Martinsson, E.; Shahjamali, M. M.; Large, N.; Zaraee, N.; Zhou, Y.; Schatz, G. C.; Mirkin, C. A.; Aili, D. Influence of Surfactant Bilayers on the Refractive Index Sensitivity and Catalytic Properties of Anisotropic Gold Nanoparticles. Small 2016, 12, 330-342.
(10) Kelly, K. L.; Coronado, E.; Zhao, L. L.; Schatz, G. C. The Optical Properties of Metal Nanoparticles: the Influence of Size, Shape, and Dielectric Environment. J. Phys. Chem. B 2003, 107, 668-677. (11) Wustholz, K. L.; Henry, A. I.; McMahon, J. M.; Freeman, R. G.; Valley, N.; Piotti, M. E.; Natan, M. J.; Schatz, G. C.; Van Duyne, R. P. Structure-Activity Relationships in Gold Nanoparticle Dimers and Trimers for Surface-Enhanced Raman Spectroscopy. J. Am. Chem. Soc. 2011, 132, 1090310910. (12) Haes, A. J.; Haynes, C. L.; McFarland, A. D.; Schatz, G. C.; Van Duyne, R. P.; Zou, S. Plasmonic Materials for Surface-Enhanced Sensing and Spectroscopy. MRS Bull. 2005, 30, 368-375. (13) Ringe, E.; McMahon, J. M.; Sohn, K.; Cobley, C.; Xia, Y.; Huang, J.; Schatz, G. C.; Marks, L. D.; Van Duyne, R. P. Unraveling the Effects of Size, Composition, and Substrate on the Localized Surface Plasmon Resonance Frequencies of Gold and Silver Nanocubes: A Systematic SingleParticle Approach. J. Phys. Chem. C 2010, 114, 12511-12516. (14) Zrimsek, A. B.; Wong, N.; Van Duyne, R. P. Single Molecule Surface-Enhanced Raman Spectroscopy: A Critical Analysis of the Bianalyte vs. Isotopologue Proof. J. Phys. Chem. C 2016, 120, 5133-5142 (15) Kleinman, S. L.; Frontiera, R. R.; Henry, A. I.; Dieringer, J. A.; Van Duyne, R. P. Creating, Characterizing, and Controlling Chemistry with SERS Hot Spots. Phys Chem Chem Phys 2013, 15, 21-36. (16) Kleinman, S. L.; Ringe, E.; Valley, N.; Wustholz, K. L.; Phillips, E.; Scheidt, K. A.; Schatz, G. C.; Van Duyne, R. P. Single-Molecule Surface-Enhanced Raman Spectroscopy of Crystal Violet Isotopologues: Theory and Experiment. J. Am. Chem. Soc. 2011, 133, 4115-4122. (17) Large, N.; Saviot, L.; Margueritat, J.; Gonzalo, J.; Afonso, C. N.; Arbouet, A.; Langot, P.; Mlayah, A.; Aizpurua, J. Acousto-Plasmonic Hot Spots in Metallic Nano-Objects. Nano Lett. 2009, 9, 3732-3738. (18) Zhang, Q.; Large, N.; Wang, H. Gold Nanoparticles with Tipped Surface Structures as Substrates for Single-Particle Surface-Enhanced Raman Spectroscopy: Concave Nanocubes, Nanotrisoctahedra, and Nanostars. ACS Appl. Mater. Interfaces 2014, 6, 17255-17267. (19) Betz, J. F.; Yu, W. W.; Cheng, Y.; White, I. M.; Rubloff, G. W. Simple SERS Substrates: Powerful, Portable, and Full of Potential. Phys Chem Chem Phys 2014, 16, 2224-2239. (20) Kurouski, D.; Sorci, M.; Postiglione, T.; Belfort, G.; Lednev, I. K. Detection and Structural Characterization of Insulin Prefibrilar Oligomers Using Surface Enhanced Raman Spectroscopy. Biotechnol. Progr. 2014, 30, 488-495. (21) Ringe, E.; Zhang, J.; Langille, M. R.; Mirkin, C. A.; Marks, L. D.; Van Duyne, R. P. Correlating the Structure and Localized Surface Plasmon Resonance of Single Silver Right Bipyramids. Nanotechnology 2012, 23, 444005. (22) Zhang, Q.; Large, N.; Nordlander, P.; Wang, H. Porous Au Nanoparticles with Tunable Plasmon Resonances and Intense Field Enhancements for Single-Particle SERS. J. Phys. Chem. Lett. 2014, 5, 370-374. (23) Mulvihill, M. J.; Ling, X. Y.; Henzie, J.; Yang, P. Anisotropic Etching of Silver Nanoparticles for Plasmonic Structures Capable of Single-Particle SERS. J. Am. Chem. Soc. 2009, 132, 268-274. (24) Rycenga, M.; Langille, M. R.; Personick, M. L.; Ozel, T.; Mirkin, C. A. Chemically Isolating Hot Spots on Concave Nanocubes. Nano Lett. 2012, 12, 6218-6222. (25) Shao, Z.; Zhu, W.; Wang, H.; Yang, Q.; Yang, S.; Liu, X.; Wang, G. Controllable Synthesis of Concave Nanocubes, Right Bipyramids, and 5-Fold Twinned Nanorods of Palladium and Their Enhanced Electrocatalytic Performance. J. Phys. Chem. C 2013, 117, 14289-14294. (26) Jing, H.; Zhang, Q.; Large, N.; Yu, C.; Blom, D. A.; Nordlander, P.; Wang, H. Tunable Plasmonic Nanoparticles with Catalytically Active High-Index Facets. Nano Lett. 2014, 14, 3674-3682. (27) Kurouski, D.; Van Duyne, R. P. In Situ Detection and Identification of Hair Dyes Using Eurface-Enhanced Raman Spectroscopy (SERS). Anal. Chem. 2015, 87, 2901-2906.
(28) Szlag, V. M.; Styles, M. J.; Madison, L. R.; Campos, A. R.; Wagh, B.; Sprouse, D.; Schatz, G. C.; Reineke, T. M.; Haynes, C. L. SERS Detection of Ricin B-Chain via N-Acetylgalactosamine Glycopolymers. ACS Sensors 2016, 1 , 842-846. (29) Bantz, K. C.; Meyer, A. F.; Wittenberg, N. J.; Im, H.; Kurtulus, O.; Lee, S. H.; Lindquist, N. C.; Oh, S. H.; Haynes, C. L. Recent Progress in SERS Biosensing. Phys Chem Chem Phys 2011, 13, 11551-11567. (30) Camden, J. P.; Dieringer, J. A.; Zhao, J.; Van Duyne, R. P. Controlled Plasmonic Nanostructures for Surface-Enhanced Spectroscopy and Sensing. Acc. Chem. Res. 2008, 41, 1653-1661. (31) Dick, L. A.; McFarland, A. D.; Haynes, C. L.; Van Duyne, R. P. Metal Film Over Nanosphere (MFON) Electrodes for Surface-Enhanced Raman Spectroscopy (SERS): Improvements in Surface Nanostructure Stability and Suppression of Irreversible Loss. J. Phys. Chem. B 2002, 106, 853860. (32) Kuncicky, D. M.; Prevo, B. G.; Velev, O. D. Controlled Assembly of SERS Substrates Templated by Colloidal Crystal Films. J. Mater. Chem. 2006, 16, 1207-1211. (33) Doherty, M. D.; Murphy, A.; McPhillips, J.; Pollard, R. J.; Dawson, P. Wavelength Dependence of Raman Enhancement from Gold Nanorod Arrays: Quantitative Experiment and Modeling of A Hot Spot Dominated System. J. Phys. Chem. C. 2010, 114, 19913-19919. (34) Haynes, C. L.; McFarland, A. D.; Zhao, L. L.; Van Duyne, R. P.; Schatz, G. C.; Gunnarsson, L.; Prikulis, J.; Kasemo, B.; Kall, M. Nanoparticle Optics: the Importance of Radiative Dipole Coupling in Two-Dimensional Nanoparticle Arrays. J. Phys. Chem. B 2003, 107, 7337-7342. (35) De Jesus, M. A.; Giesfeldt, K. S.; Oran, J. M.; Abu-Hatab, N. A.; Lavrik, N. V.; Sepaniak, M. J. Nanofabrication of Densely Packed Metal–Polymer Arrays for Surface-Enhanced Raman Spectrometry. Appl. Spectrosc. 2005, 59, 1501-1508. (36) Félidj, N.; Aubard, J.; Lévi, G.; Krenn, J. R.; Hohenau, A.; Schider, G.; Leitner, A.; Aussenegg, F. R. Optimized Surface-Enhanced Raman Scattering on Gold Nanoparticle Arrays. Appl. Phys. Lett. 2003, 82, 3095-3097. (37) Zhang, M.; Large, N.; Koh, A. L.; Cao, Y.; Manjavacas, A.; Sinclair, R.; Nordlander, P.; Wang, S. X. High-Density 2D Homo- and Hetero- Plasmonic Dimers with Universal Sub-10-nm Gaps. ACS Nano 2015, 9, 9331-9339. (38) Le, F.; Brandl, D. W.; Urzhumov, Y. A.; Wang, H.; Kundu, J.; Halas, N. J.; Aizpurua, J.; Nordlander, P. Metallic Nanoparticle Arrays: A Common Substrate for Both Surface-Enhanced Raman Scattering and Surface-Enhanced Infrared Absorption. ACS Nano 2008, 2, 707-718. (39) Bernard, S.; Felidj, N.; Truong, S.; Peretti, P.; Levi, G.; Aubard, J. Study of LangmuirBlodgett Phospholipidic Films Deposited on Surface Enhanced Raman Scattering Active Gold Nanoparticle Monolayers. Biopolymers 2002, 67, 314-318. (40) Seitz, O.; Chehimi, M. M.; Cabet-Deliry, E.; Truong, S.; Felidj, N.; Perruchot, C.; Greaves, S. J.; Watts, J. F. Preparation and Characterisation of Gold Nanoparticle Assemblies on Silanised Glass Plates. Colloids Surf., A 2003, 218, 225-239. (41) Kurouski, D.; Large, N.; Chiang, N.; Greeneltch, N.; Carron, K. T.; Seideman, T.; Schatz, G. C.; Van Duyne, R. P. Unraveling Near-Field and Far-Field Relationships for 3D SERS Substrates - A Combined Experimental and Theoretical Analysis. Analyst 2016, 141, 1779-1788. (42) Yu, Q.; Guan, P.; Qin, D.; Golden, G.; Wallace, P. M. Inverted Size-Dependence of Surface-Enhanced Raman Scattering on Gold Nanohole and Nanodisk Arrays. Nano Lett. 2008, 8, 19231928. (43) Dieringer, J. A.; McFarland, A. D.; Shah, N. C.; Stuart, D. A.; Whitney, A. V.; Yonzon, C. R.; Young, M. A.; Zhang, X.; Van Duyne, R. P. Surface Enhanced Raman Spectroscopy: New Materials, Concepts, Characterization Tools, and Applications. Farad. Discuss. 2006, 132, 9-26. (44) Liao, P. F.; Bergman, J. G.; Chemla, D. S.; Wokaun, A.; Melngailis, J.; Hawryluk, A. M.; Economou, N. P. Surface-Enhanced Raman Scattering from Microlithographic Silver Particle Surfaces. Chem. Phys. Lett. 1981, 82, 355-359.
(45) Chen, C. Y.; Burstein, E. Giant Raman Scattering by Molecules at Metal-Island Films. Phys. Rev. Lett. 1980, 45, 1287-1291. (46) Stiles, P. L.; Dieringer, J. A.; Shah, N. C.; Van Duyne, R. P. Surface-Enhanced Raman Spectroscopy. Annu. Rev. Anal. Chem. 2008, 1, 601-626. (47) Kurouski, D.; Postiglione, T.; Deckert-Gaudig, T.; Deckert, V.; Lednev, I. K. Amide I Vibrational Mode Suppression in Surface (SERS) and Tip (TERS) Enhanced Raman Spectra of Protein Specimens. Analyst. 2013, 138, 1665-1673. (48) Brown, R. J.; Milton, M. J. T. Nanostructures and Nanostructured Substrates for SurfaceEnhanced Raman Scattering (SERS). J. Raman. Spectr. 2008, 39, 1313-1326 (49) Gunnarsson, E. J.; Bjerneld, H.; Xu, S.; Petronis, B.; Kasemo, B.; Kall, M. Interparticle Coupling Effects in Nanofabricated Substrates for Surface-Enhanced Raman Scattering. Appl. Phys. Lett. 2001, 78, 802-804. (50) Atay, T.; Song, J.-H.; Nurmikko, A. V. Large Enhancement of Fluorescence Efficiency from CdSe/ZnS Quantum Dots Induced by Resonant Coupling to Spatially Controlled Surface Plasmons. Nano Lett. 2004, 2004, 1627-1631. (51) Greeneltch, N. G.; Blaber, M. G.; Henry, A. I.; Schatz, G. C.; Van Duyne, R. P. Immobilized Nanorod Assemblies: Fabrication and Understanding of Large Area Surface-Enhanced Raman Spectroscopy Substrates. Anal. Chem. 2013, 85, 2297-2303. (52) McFarland, A. D.; Young, M. A.; Dieringer, J. A.; Van Duyne, R. P. WavelengthScanned Surface-Enhanced Raman Excitation Spectroscopy. J. Phys. Chem. C 2005, 109, 11279-11285. (53) Lumerical Solutions, I.: http://www.lumerical.com/tcad-products/fdtd. (54) Lynch, D. W.; Hunter, W. R.: An Introduction to the Data for Several Metals. In Handbook of Optical Constants of Solids; Palik, E. D., Ed.; Academic Press, Burlington, MA, 1997; Vol. 1; pp 275-367. (55) Johnson, P. B.; Christy, R. W. Optical Constant of Noble Metals. Phys. Rev. B 1972, 6, 4370–4379. (56) Masango, S. S.; Hackler, R. A.; Large, N.; Henry, A.-I.; McAnally, M. O.; Schatz, G. S.; Stair, P. C.; van Duyne, R. P. High-Resolution Distance Dependence Study of Surface-Enhanced Raman Scattering Enabled by Atomic Layer Deposition. Nano Lett. 2016, 16, 4251-4259. (57) Ringe, E.; Langille, M. R.; Sohn, K.; Zhang, J.; Huang, J.; Mirkin, C. A.; Van Duyne, R. P.; Marks, L. D. Plasmon Length: A Universal Parameter to Describe Size Effects in Gold Nanoparticles. J. Phys. Chem. Lett. 2012, 3, 1479-1483. (58) Ringe, E.; Sharma, B.; Henry, A. I.; Marks, L. D.; Van Duyne, R. P. Single Nanoparticle Plasmonics. Phys Chem Chem Phys 2013, 15, 4110-4129. (59) Zuloaga, J.; Nordlander, P. On the Energy Shift Between Near-Field and Far-Field Peak Intensities in Localized Plasmon Systems. Nano Lett. 2011, 11, 1280-1283.
Figure 1. SEM images of SP-FONs (A, B) and ST-FONs (C, D). Scale bars correspond to 200 nm (A, B) and 300 nm (C, D). (E) Size distributions of nanofeatures on the top (upper panels) and side (lower panels) surface of SP- and ST-FONs. 41x60mm (300 x 300 DPI)
Figure 3. FDTD calculations for the ST- and SP-FONs. (A, B) Modeled geometries used in the FDTD simulations for the Au ST-FON and Ag SP-FON, respectively. (C, D) Reflectance spectra (dotted lines) and fourth power of the near-field (|E/E0|4, solid line) calculated within the gap (white mark in panels E and F) for the Au ST-FON and Ag SP-FON, respectively. (E, F) Spatial distribution of |E/E0|4 around the Au ST-FON (λ=810 nm) and Ag SP-FON (λ=800 nm), respectively. 150x83mm (300 x 300 DPI)
Figure 4. FDTD calculations for the SP- and ST-FONs. (A, B) Modeled geometries used in the FDTD simulations for the Au SP-FON and Ag ST-FON, respectively. (C, D) Reflectance spectra (dotted lines) and fourth power of the near-field (|E/E0|4, solid line) calculated within the gap (white mark in panels E and F) for the Au SP-FON and Ag ST-FON, respectively. (E, F) Spatial distribution of |E/E0|4 around the Au SP-FON (λ=700 nm) and Ag ST-FON (λ=725 nm), respectively. 150x83mm (300 x 300 DPI)